4 MECHANICAL TEST METHODS FOR LAMINA 4.1 Introduction Birefringent coatings, holography, anisotropic photoelasticity, and Moir6 have been successfully used in experimentally evaluating composite materials. Topics relating to experimental procedures and laminate test methods are available in texts [ 13], or from periodic publications. The discussions presented herein focus on methods used to establish mechanical and physical properties of orthotropic lamina. Many test procedures and specimen geometries used with isotropic materials are not applicable to composites. For composites, one is generally concerned with defining load and displacement (or strain) histories throughout a specific test sequence using LVDTs, extensometers, or strain gages. An LVDT or extensometer (using optical or electrical resistance strain gages) measures the relative displacement between reference points on a specimen, and the sensing elements of either device are not directly applied to the specimen. An electrical resistance strain gage can be applied directly to the specimen. Information from each of these devices is processed to define the parameter(s) of interest. Procedures for accomplishing this are discussed in texts such as Dally and Riley [4] and is not presented herein. Strain gages are perhaps the most commonly used strain measuring device and are briefly discussed.
4.2 Strain Gages Applied to Composites The concept behind electrical resistance strain gages is simple and is based on the original 1856 findings of Lord Kelvin [4], who found that the resistance of copper and iron wires increased as tensile loads were applied to each. Since the applied loads caused changes in the original length of each wire, which are expressible as strains, a direct correlation between strain and resistance change is obtainable. The evolution of strain gage technology from the first practical application in 1938 by the separate efforts of Ruge and Simmons has been substantial. There are many 102
Mechanical Test Methods for Lamina
103
factors which can cause errors in correlating resistance change to strain, and they can be grouped into six categories [3]" (a) The wire must be firmly bonded to the specimen so that its deformation accurately represents the deformation in the specimen. (b) The wire must not locally reinforce the structure. If it does, the deformation of the wire does not accurately reflect specimen deformation. (c) The wire must be electrically insulated from the structure. (d) The change in wire resistance per unit microstrain is generally small, but must be accurately measured. (e) Deformation of the structure via mechanisms other than applied loads (such as temperature) must be accounted for. (f) Aggressive environments may cause oxidation of the wire and lead to resistance changes of the wire which cause erroneous results. The selection of an appropriate strain gage for a specific application is not a trivial matter, and issues such as temperature compensation, working environment and appropriate strain measuring circuits must all be considered for accurate collection and evaluation of data. These topics are beyond the scope of this text, but are addressed in various references [39].
4.2.1 General Interpretation of Strain Gage Data A single element strain gage applied to a uniaxial tension specimen is represented in Figure 4.1. The longitudinal axis of the gage defines the direction in which strains are measured. Although a uniaxial state of stress exists, a state of biaxial strain results. Both axial and transverse specimen strains affect the strain measured by the gage. The relation between resistance change and a general state of strain is written as [4] AR ........ " Sa•a "1" StEt "~ SsYat (4.1) R where AR R Sa St Ss
= = = " = ea = et = )/at =
change in gage resistance original gage resistance sensitivity of the gage to axial strains sensitivity of the gage to transverse strains sensitivity of the gage to shear strains normal strain in the axial direction of the gage normal strain in the transverse direction of the gage shear strain
r
t Figure 4.1. Single element strain gage on a uniaxial tension specimen.
104
Laminar Composites
In general, the sensitivity of a strain gage to shear strain is small and therefore neglected. A parameter called the transverse sensitivity factor is introduced into equation (4.1) and is K = St/Sa (4.2) The numerical values for K generally range from 0.05 to 0.05, and manufacturers report these numbers as percents, so that K  5% corresponds to K = 0.05. Using this definition of transverse sensitivity, and setting Ss = 0, equation (4.1) becomes AR R
 Sa (Ca + Ket)
(4.3)
A calibration constant known as the gage factor Sg (supplied with each strain gage) relates the resistance change to the axial strain by AR/R = Sgea. The calibration constant is determined from a test performed on each lot of gages being produced. This test is conducted by mounting a gage on a standardized beam, so that its longitudinal axis coincides with the direction of maximum normal strain when the beam is deflected a specified amount. The state of stress at the gage location is uniaxial tension, but a state of biaxial strain exists in which et = V0ea; where v0 is Poisson's ratio of the calibration beam (generally v0 = 0.285). Substituting this into equation (4.3) results in AR R = Saea(1  voK)
(4.4)
From this expression the gage factor can be defined as Sg =
zXR/R Ea
= Sa(1  voK)
(4.5)
The strain experienced by the gage (in its longitudinal direction) is related to the resistancechange by ea =
AR/R Sg
(4.6)
Equation (4.6) is based on the following assumptions: (1) the gage is subjected to a uniaxial stress field; (2) the gage grid is parallel to the direction of the stress field; and (3) the gage is mounted on a material for which v = u0 used in the calibration test. If all of these assumptions are satisfied, the measured strain (era) is identical to Ca. This ideal situation seldom exists, and in general equation (4.6) should not be used directly. Although erroneous results obtained by direct application of equation (4.6) are not severe in many situations involving isotropic materials, they can be when considering composite materials. The percent error associated with using equation (4.6) directly has been established [4] and is E =
K(et/ea + vo) (100) 1 voK
(4.7)
The relationship between E and K for various Et/Ea ratios are presented in Figure 4.2. The ratio of transverse to axial strain (et/ea) is established from the loading conditions which produce the strain to be measured. The errors should
M e c h a n i c a l Test M e t h o d s for L a m i n a
30
25 L
=o 20 I__ uJ t15 O (i,1
13.
10
i , , ,

I ' ' ' '
gr.
/ Ea
I'
'''
I
'
'
'
'
I ''i
'
'
'
I
,
,
,
105
 0
.......... Et./ga = 1
. . . . . et/ea = 4
..'"'""
5 , 0 .6~'~'r, 0.00 0.01
,7"~,,
I
,
..
~
0.02
I
,,
,,
0.03
,
0.04
0.05
Transverse Sensitivity Factor
Figure 4.2. Percent error associated with various transverse sensitivi~s and 8t/Sa ratios (after Dally and Riley [4]).
be estimated from equation (4.7) with an estimated ratio of et/ea based on the material being tested. In order to compensate for the effects of transverse sensitivity, a minimum of two strain measurements is required. Assuming that a biaxial strain gage rosette is used (two strain gages mounted on a specimen so that two orthogonal strains are measured), the true strain in the x and y directions can be established from the measured strains [4]. Denoting ex and ey as the true strains, and emx and Emy a s the measured strains, respectively, the following relationships are obtained:
ex =
(1  voK)(emx  Kemy) 1 K2
ey =
(1  voK)(emy  Kemx) 1  K2
(4.8)
These expressions for the biaxial strain gage rosette are only applicable for that particular type of rosette. A variety of other types of strain gage rosette are available. Two of these often used with composites are the rectangular and delta rosettes (each containing three strain gage elements). These are schematically shown in Figure 4.3. Relationships between measured and true strains for the rectangular rosette are given in Pendleton and Tutfle [3] as ~X  "
ey =
(1  voK)(emx  Kemy) 1  K2 (1  voK)(emy  Kemx) 1  K 2
(4.9)
voK) 1  K 2 {em45  K(emx + emy  em45)
(1 
e45 =
where em45 is the measured strain for the 45 ~ strain gage. For the delta rosette the relationships between true and measured strains are 1voK {( 3) Ex " 1  K 2 1+
emx 
2Kem6~176 3
106
Laminar Composites
Y
Y
X
X
X
Biaxial
Rectangular
Delta
Figure 4.3. Biaxial, rectangular; and delta strain gage rosettes.
11)oK { (1K ) 1  K2 + ~
e6o = El20

em60 2K
Emx+Eml20 /
(4.10)
3
1voK { ( K ) + Em6O} 1 K 2 1 ~ ~ eml20 2K emx 3
Equations (4.8) to (4.10) are only valid if K is identical for each gage. For situations in which K varies from gage to gage, the appropriate relations can be found in a technical note [10]. The Cartesian strain components associated with each of these true strains are obtained from the strain transformation equation in Chapter 2. The typically low values of K that strain gage manufacturers can obtain indicate that measured strain gage data generally yields accurate results. This is true in many cases involving isotropic materials; it is not generally true for composite materials. Transverse sensitivity effects for composites are typically enhanced since the apparent Poisson's ratio for a orthotropic material is generally different from the v0 of the gage calibration material. The evaluation of transverse sensitivity effects for strain gages on composites presented by Tuttle [11] is summarized in equation (4.3). Tests were conducted on unidirectional carbon/epoxy specimens subjected to uniaxial tension. Both axial and transverse strain gages with K = 0.03 were used, and fiber orientations varied. The axial gage had at most a 1% error between measured and corrected data for the worst case (fiber orientation greater than approximately 70~ The transverse gage, however, was shown to exhibit severe errors when K was not used to correct the measured strain gage data. Results of the analysis described in Pendleton and Tuttle [3] are presented in Figure 4.4, 0 ~.
50
n
100 150
~
200
250
0
I 10
I 20
I,
I
30
40
I ..... 1..... I 50 60 70
I 80
I 90
Fiber Angle (degrees)
Figure 4.4. Percentage error in measured transverse strain (without correcting for K) vs 0 (after Pendleton and Tattle [3]).
Mechanical Test Methods for Lamina
107
where it is seen that the percent error resulting from neglecting K is large. The magnitude of the measured strains for the transverse gage are considerably lower than the axial strains, but the errors are significantly higher. E x a m p l e 4.1. Assume that a delta rosette (K = 0.05 for each gage) is applied to
a unidirectional composite. The strain gages shown in Figure E4.1 indicate strains of eA = 23,015 ~tin/in, eB = 22,307 Ixin/in, and ec =  9 9 3 6 ~tin/in. Neglecting transverse sensitivity, the strains for each gage are e0 = ex cos 2 0 + eysin20 + Yxy sin 0 cos 0, which results in eB ec
=
(23o15) 22,307 9936
1 cos 260 cos 2 120
x10 6=
Solving this expression yields
{
e,y )'xy

0 sin 260 sin 2 120
o
sin 60 cos 60 sin 120 cos 120
ey Yxy
(23,o15) 576 37,232
x 10 6
Y
60 ~ C
B 60~
l A
•
Figure E4.1. Delta strain gage rosette orientation.
Using the measured strain (CA, etc.) and equation (4.10) with K = 0.05 and vo = 0.285, the true strain for each gage is ex } [ 1.0040 eto =  0 . 0 3 2 9 e12o 0.0329
0.0329 1.0040 0.0329
00329]{23015){ 227 ) 0.0329 1.0040
22,307 9936
=
21,966  11,467
x 10 6
These strains, when used to evaluate the Cartesian strain components, result in ex }
eto 8120
[ =
1.0040 0.0329 0.0329
0.0329 1.0040 0.0329
oo329](23o15}( 227 }
0.0329 1.0040
22,307 9936
=
21,966  11,467
x 10 6
A direct comparison between these results and those for K = 0.0 shows an error of 3.5% in the worst case for ex and Yxy, but a substantial error exists for ey.
4.2.2 Strain Gage Misalignment For an isotropic material the effects of poor alignment are not as critical as for a composite. For example, using a steel specimen and allowing a set of biaxial
108
Laminar Composites
gages to be misaligned by some angle (/~), as shown in Figure 4.5, results in errors for both the axial and transverse gages. In Pendleton and Tuttle [3], results for a gage misalignment o f   4 ~
G
t:I
! "
I
Figure 4.5. Gage misalignment on an isotropic specimen. For a composite both the misalignment (t3) and fiber orientation angle (0) contribute to the errors in strain gage measurement. In Tuttle and Brinson [12], tests on the effects of strain gage misalignment as a function of fiber orientation were investigated for the specimen shown schematically in Figure 4.6. The percentage error in axial and transverse gages which resulted were reported in Pendleton and Tuttle [3] to be similar to those shown in Figures 4.7 and 4.8, respectively. The transverse gage experienced the most severe errors. Situations often arise in which the complete state of strain is required, a single element strain gage, or a biaxial rosette are not adequate. A strain gage rosette in which three normal strains are determined is recommended for such cases. The transverse sensitivity corrections for rectangular and delta rosettes expressed by equations (4.9) and (4.10), respectively are applicable in this case. Proper alignment of strain gages on composite can be critical when defining a complete state of strain, and care should be taken to ensure proper alignment.
I Figure 4.6. Gage misalignment on a composite specimen.
4.2.3 Strata Gage Reinforcing Effects Strain gages applied directly to a specimen have been shown to produce reinforcement errors in tests with low modulus materials such as plastics [1316]. It is possible that similar reinforcement effects occur in composites. Strain gage reinforcement is most likely to occur in regions where the geometric crosssection of the specimen is thin and the elastic modulus in the gage direction is low. The normalized variation of Ex, as defined by equation (3.19), with respect to the minimum elastic modulus of the material (E2) decreases rapidly with increasing
Mechanical Test Metkods for LwnL.m 30 =.. 2 ,~
20

I~ =  2
~


13 =4
~

10 . ,
,' . . . . .
'O
"'.
" .......
.........
13= +2 ~
~
/
" " , .
.
.
.
109
p=+4 ~ 
.
.,.
o,
~. lO 2O
30
0
10
20
30
40
50
60
70
80
90
Fiber Angle (degrees)
Figure 4. 7. Percent error in axial gage (after Pendleton and Tuttle [3]).
I
~ool/ sol.
= uJ
I
~)~ a.
0
, ...... ,
,
,
,
,
. /
. . .~. . . .. .
_
..,,..,. ....
""
_,......._,
~
~
..,,.. .
f
P =4~ t o ....P =+2~ /  z x  P = ~ ~ i .
.
.
. .................................................. ,' ~"~"(~.~~'"... T x"O~~,~O...OOO"~O'"O''O'O'O'"O"O'"O"O"O
100 / 0
I, 10
I 20
I 30
I 40
I 50
I 60
I 70
I 80
/ 90
Fiber Angle (degrees)
Figure 4.8. Percent error in transverse gage (after Pendleton and Tuttle [3]). 5
'1''''1''
''1''''
4 3 LU
2
1 0 ,,,,I,, 0 10
,,I,,,,I,,,,I 20 30
.... 40
I .... I,,,,I,, 50 60 70
,,I,,,, 80
90
Fiber Orientation Angle (degrees)
Figure 4.9. Variation of Ex ]E2 with fiber orientation.
fiber orientation as shown in Figure 4.9 for Scotchply 1002 glass/epoxy. The magnitudes of Ex/E2 differ for other material systems, but the trend is the same. For fiber orientations of 30~ 0 < 30 ~ Ex > 2E2, while for all other fiber orientations Ex < 2E2. This can influence the degree to which a strain gage will reinforce a specimen and provide inaccurate measures of the actual strain. In many practical situations the strain gage is unlikely to significantly reinforce the composite. Given the wide range of possible material properties available with
I I0
Laminar Composites
composites, there is a possibility that strain gage reinforcement can affect test results. Methods of accounting for the reinforcing effect of strain gages are available [3]. The procedure consists of establishing a set of correlation parameters from tests on a calibration specimen, and subsequently relating them to the measured strains on the actual specimen. A simple model for estimating the amount of fiber reinforcement can be defined following the procedures in Dally and Riley [4] for birefringent coatings. The simplest case to evaluate is uniaxial tension. Assume a unidirectional lamina has a single element strain gage applied to its surface in the direction of the applied state of stress (trx) as shown in Figure 4.10a. Assume the gage is perfectly bonded to the specimen, there are no stress concentrations at the specimen/gage interface, and the load sharing between the gage and specimen can be modeled as shown in Figure 4.10b.
gage ,
sPecime n _. ~
Ox
[   hg
specimen (~x
axs (a)
(b)
Figure 4.10. Model of load sharing between specimen and strain gage for uniaxial tension.
In this figure trxu is the axial stress in the ungaged region of the specimen. Stress trxs and trxg represent the axial stresses in the specimen and gage, respectively. The thicknesses of the specimen and gage are represented by hs and hg. Assuming the representative volume element associated with Figure 4.10b has a width dy, a force balance in the xdirection results in hstrxudy = hsoxs dy + hgtrxgdy. Therefore, trxu = Crxs+
trxg
(4.11)
The relationship between axial strain and stress is established from equation (3.15). Although reinforcement effects may occur transverse to the applied load, the major reinforcement will be in the direction of load application. The relationship between applied stress and strain in the ungaged region of the specimen is =
~xu
= Exsexs
The specimen and gage stresses are defined by trxs = Exsexs, and Orxg"Eg6xg, respectively. Using the assumption that the specimen and gage experience the same strain (exg = exs), equation (4.11) becomes
hg  1] exg exu = [l + ~EgS1
Mechanical Test Methods for Lamina
111
The ratio of specimen to gage thickness can be represented as n = hs/hg. Introducing this into the preceding equation, and rearranging it in order to relate the axial strains in the ungaged region of the specimen to those in the gaged region, results in
exu =
(  ) 1 + SllEg
Exg
(4.12)
n
The greatest reinforcement effect results when S ll is a maximum, which generally occurs at fiber orientations of 90 ~. For this case equation (4.12) can be expressed as exu =
1+
(4.13)
exg The degree of reinforcement (exu/exg) depends on the composite material, strain gage material, and the ratio of specimen to gage thickness (n = hs/hg). A strain gage can be characterized as a plastic, so Eg is typically less than E2. Evaluating equation (4.13) for various Eg/E2 ratios as a function of hs/hg results in the distribution shown in Figure 4.11, where it is obvious that the effect of strain gage reinforcement decreases rapidly with increasing hs/hg. It appears as if substantial reinforcement is present for a large range of hs/hg, but strain gages are generally on the order of 0.0035 in thick. Therefore, at hs/hg = 10, the specimen would be 0.035 in thick. One should evaluate exu/exg from either equations (4.12) or (4.13) to determine if possible errors warrant compensation.
10 
I
I
I
I
I
i
. i., ,_t.. _,, ~.
....
r../t:::~g/t"2 = 0.5 E g / E 2 = 1.0
4 , "~
....
Eg/E 2 = 2.0
6 :3
:
'~
0
0
I
I
I "
I
I
I
i
I
I
I
I
I
1
2
3
4
5
6
7
8
9
10
hs/hg
Figure 4.11. Strain gage reinforcement effects for uniaxial tension. Strain gage reinforcement is more pronounced when flexure stresses exist. Assume a unidirectional composite lamina is subjected to pure bending. The strain variation through the specimen (exs) and strain gage (exg) in the region containing the gage are modeled in Figure 4.12. The distance d is used to define the location of the neutral bending axis. The strain gage is assumed to be isotropic, and the stresses in the gage and specimen are expressed as trxg = Egexg and trxs = Exsexs = exs/S11, respectively. Since the m
112
Laminar
Composites Z ~ ....
[',,age:.:
9
........
": .
.
.
.
.
.
.
exg for d <_. z <__(d
hs
~

+ hg)
Sxs for (d  hs) _< z _< d
_ ~ eSxs
M
Figure 4.12. Model for strain gage reinforcement due to pure bending.
specimen is subjected to pure bending, the strains are related to the radius of curvature by e~s=
Z
fordhs
P Z
exg = P
ford
Satisfying the condition of equilibrium of forces in the xdirection requires
fd d trxs d z + [d+hg Crxgd z = hs Jd
0
Using equation (4.14) in the expressions for axs and trxg results in
Exs fd d (z/p) dz + Eg [d+hg (z/p) dz = 0 h~ Jd Evaluation of these integrals yields an explicit definition of the neutral bending axis location d as a function of material properties and thickness of constituent materials: d  Exsh2  Egh2 (4.15) 2[Exsh2 Jr" Eghg] The ratio of specimen to gage thickness (n = hs/hg) can be introduced into this expression as it was for the case of uniaxial tension, which allows equation (4.15) to be expressed as d = Clhg (4.16) where
Exs n2  Eg Cl  2[Exsn + Eg] The radius of curvature is determined by establishing the standard conditions d Ztrxsdz + fJ+hg Ztrxg dz = 0. Using of equilibrium for moments from M = fdh, equation (4.14)
l i p [Exs fahsa
in
Z2dz
the
expressions
+ Eg fj+hg
Z2 dz].
for
trxs and
trxg results
in
M =
Upon evaluation of these integrals, it is
Mechanical Test Methods for Lamina
113
convenient to define two additional terms: C2 = 3 d 2 h s  3dh2s + h 3
(4.17)
C3 = 3d2hg + 3dh~ + hg3 where d is defined by equation (4.16). The curvature and bending moment in the strain gaged area are related by (1/p)g = 3M/(ExsC2 + EgC3). For an unreinforced specimen the relationship between curvature and moment is easily established since hg = 0, d = hs/2, and crxg = 0. The resulting relationship is (1/P)u = 12M/E~sh 3. Since exg = Z/pg and exu = Z/pu, the ratio of strains in the ungaged region to those in the gaged region is exu/exg = Pg/Pu. Using the relationships for (1/p)g and (1/p)u results in
exu = 4{ExsC2 + EgC3} 6xg Exsh3s where
C2
(4.18)
and C3 are defined by equation (4.17).
Equation (4.18) is more complex than either (4.12) or (4.13) because of the relationships between C2, C3, d, and the relative thickness of both specimen and gage. The maximum reinforcing (exu/exg) will generally occur for fiber orientations of 90 ~ with respect to the xaxis (in the x  y plane). Expressing equation (4.18) in terms of the elastic constants Eg and E2 is not warranted for this case because of coupling of terms related through d. Evaluating equation (4.18) for various ratios of hs/hg and Eg/E2 produces the results shown in Figure 4.13. At hs/hg = 10 the best case shown (Eg/E2 = 0.5) predicts exu/exg = 1.17, which implies a 17% stiffening effect. As with uniaxial tension, the possibility of gage reinforcement from bending should be evaluated prior to strain gage application. 10
i"t
,
1'.
I
I
I
~.\
,~,i,p..]"
t 1
I
!
I
L; Eg/E2 = 0.5 ..,e,. Eg/E2= 1.0 O. Eg/E2 2 0
~'~.
0
,,
i ,.,
\ ",
6
I
I 2
I 3
I 4
,,, I 5
I, 6
I,, 7
_
1 8
I 9
10
hs/hg
Figure 4.13. Strain gage reinforcement effects for flexure in the range 0 <_hs/hg <_ 10. The amount of reinforcing associated with a specific set of gage and specimen properties can be estimated from equation (4.12) or (4.18). If reinforcement is considered a potential problem, the procedures in Pendleton and Tuttle [3] can be used.
114
Laminar Composites
4.3 Experimental Determination of Mechanical Properties Nine independent elastic constants are required to define the mechanical response of an orthotropic lamina. In many cases of practical importance a state of plane stress exists and the outofplane material properties are not required since they are often approximated by inplane properties (E2 = E3, etc.). The mechanical properties generally considered to be of greatest interest are El, E2, G12, v12, and v21. Lamina failure strengths can be established as part of the experimental procedures used for determining elastic properties. A unidirectional laminate is typically used since individual lamina are too thin and weak in the transverse direction to sustain sufficient load for determining elastic moduli and failure strength. The procedures discussed herein are those most commonly used in establishing the properties just identified, and those which are typically easiest to implement.
4.3.1 Tensile Testing Each previously cited material property can be established from uniaxial tension tests of unidirectional laminates. Although G l2 can be established from uniaxial tension tests, discussion of shear modulus determination is reserved for a later section. The recommended test procedures which should be followed in establishing these properties are described in ASTM D303976. A dogbone specimen used in uniaxial tension tests of flat coupons for isotropic materials is not acceptable for laminates. Establishing E1 and E2 (along with v12 and v21) requires test specimens with fiber orientations of 0 ~ and 90 ~ respectively. A dogboneshaped specimen with a 0 ~ fiber orientation will result in the formation of matrix cracks parallel to the fibers, and an eventual failure in the region indicated in Figure 4.14. A stressstrain curve generated from such a specimen may contain a region of valid data (up to the point where the matrix cracks begin to develop), but will generally not yield an accurate modulus prediction or failure strength.
failure cracks
Figure 4.14. Failure mechanism for composite dogbone specimen. The 90 ~ specimen will not fail in this manner. Damage induced by machining the specimen into a dogbone shape may weaken the matrix to the extent that invalid predictions of E2 result. A more appropriate specimen is a fiat coupon with end tabs. The end tabs help reduce the probability of failure in the grip region where the applied loads are transferred from the testing machine to the specimen. Without end tabs the normal force between the specimen and grips could crush the fibers in the grip region and produce premature failure. The standard dimensions of a test specimen depend on fiber orientation. The geometry and dimensions for 0 ~ and 90 ~ tensile coupons are given in Figure 4.15. The
Mechanical
Test Methods
for Lamina
115
Specimen Geometry
t
,
I
W ,
i
N'',,~'~',''~'', ...
i , J
~,
.
.
.
,~ ,, '~ '~ ', 9 ,~ . ', ~. ~. f "1 .
.
.
.
.
.
.
.
.
.
.
al
~,
9
I ,
!
60 ~
Figure 4.15. Geometry and dimensions of O* and 90~ tensile specimens.
: ll, llli,,tillljIzilllil i !i
G2
ea
gives E1 & F,t/Ea gives v12
ea
gives E2 & s
,,,.._ v
gives V21
Figure 4.16. Schematic of f~er orientations and strain gage positioning for determining El, E~ V12, and V21. total thickness of a specimen depends on the number of plies in the laminate. The end tabs are typically 1.50 in long and 0.125 in thick. The tabs are beveled to allow for a more uniform load transfer from the grips to the specimen. Strain gages or extensometers are often used to determine the stressstrain history of a specimen. Using both longitudinal and transverse gages, a single test can produce either El, v]2 or E2, v2], depending upon fiber orientation, as illustrated in Figure 4.16. Strain gages placed on the front and back of each specimen (in a full Wheatstone bridge) negate the effects of bending due to eccentricity of the load line [4]. A biaxial extensometer could also be used. Specimen Dimensions ,
,
H
,
Fiber Orientation
Width (in)
Number of Piles
Length (in)
00 90 ~
0.50 1.00
68 816
9.00 9.00
A typical set of stressstrain curves for 0 ~ and 90 ~ AS/3502 graphite/epoxy tensile specimens is presented in Figure 4.17. Failure of the 90 ~ specimen is matrix dominated. The fibers are capable of sustaining a far greater load than the matrix; therefore, the 00 specimen fails in a significantly different manner. Along the failure surface there are jagged edges indicating that failure was not
116
Laminar Composites 250
i
,
l
i
l
'
i
l'
",'
I
10
'i
200 . m
W
150 .=
ffj .~ 100
?i'
50
0
I
0
5000
10000
t
0
0
Axial Strain (minfin)
5000
10000
Axial Strain (min/in)
Figure 4.17. Stressstrain curves for AS/3502 graphite~epoxy.
instantaneous. As the ultimate load is approached, individual fibers begin to fail with an audible "ping" sound. Individual fibers will fail at slightly different load levels.
4.3,2 Compression Testing In conducting compression tests it has been noted that a composite material may exhibit different tensile and compressive moduli (El, E2, etc.) and is termed bimodMar. The influence of bimodularity on analysis techniques and failure analysis can be significant [17]. The failure strength is generally considered more significant than modulus when comparing tensile and compressive behavior. Some of the differences between tensile and compressive behavior can be attributed to the difficulty of compression testing. Slight geometric variations in the specimen may result in eccentric loads, which enhance the possibility of failure due to instability as opposed to stress. There are three accepted test methods that reduce this possibility as described in Whitney et al. [1]. Each is briefly outlined and schematic diagrams of grip arrangements are presented. Strain gages are generally used for each of these test methods. Additional compression test methods are available, which are presented in a survey article pertaining to compression testing of composites [18]. Type I. This method is characterized by having a completely unsupported specimen with a relatively short test section length. Several types of fixtures exist for this method. The Celanese (ASTM D341075) test fixture and associated specimen geometry are shown in Figure 4.18. The Illinois Institute of Technology Research Institute (UTRI) [19] test fixture uses a test specimen identical to the Celanese fixture and is shown in Figure 4.19. Strain gages are mounted on the specimen, which is loaded through serrated wedges constrained by solid steel bases. The Northrop test fixture [20] is simpler than the Celanese or IITRI fixtures and is shown in Figure 4.20. The final example of Type I compression testing is
Mechanical Test Methods for ~
~ y
117
mUot
strain gage
~ /specimen
cylindrical shell
A
Figure 4.18. Celanese test fixture and specimen (ASTM D 3410.75). fixture
specimen "
i
! J D
! I
'
!
Figure 4.19. Modqied grips for HTRI compression test [19].
1
~t 1 Ol
!
IO]
[o~ Figure 4.20. Northrop compression test specimen and fixture [20]. the NBS (National Bureau of Standards) test fixture [21]. This fixture combines aspects of the Celanese and IITRI fixtures and adds features that allow for tensile tests. The NBS fixture is shown in Figure 4.21. All four of the Type I test methods yield acceptable results, but are difficult to conduct because of load line eccentricity.
118
Laminar
Composites
specimen fixture
Figure 4.21. NBS compression test specimen and fixture [221. Type lI. In this class of tests the specimens are characterized as having a relatively long test section that is fully supported. The SWRI (Southwest Research Institute) [22], and the Lockheed type fixtures [23] are schematically shown in Figures 4.22 and 4.23, respectively. Results from experiments using these grips are comparable to data from Type I tests. The SWR/grip has a cut in one support to allow for a transverse gage to measure Poisson's ratio in compression. Longitudinal strain is measured by an extensometer or strain gage placed on the edge of the specimen. The specimen is a modified tensile specimen in which the overall length is reduced while the end tab lengths are increased. The entire specimen length is supported by the fixture. The Lockheed fixture uses side supports only over the gage section of the specimen, which is the primary difference between it and the SWRI fixture. fixture
specimen
J i o
o
]
i
m i
I /
i
Figure 4.22. SWRI compression test fixture [221. Type IlL The final class of compression test methods involves two sandwich beam specimen configurations. In each case straightsided coupons are bonded to a honeycomb core, which supplies lateral support. The elastic moduli and Poisson's ratio are determined from relationships between applied loads and strain gage readings taken from the specimen [ 1]. Results of failure strengths from this method are usually higher than those from the other methods. The sandwich beam method can also be used to determine tensile properties [24]. The two specimen configurations
M e c h a n i c a l Test M e t h o d s for L a m i n a
119
Ill rllrrll ill r'T
o
_
o]
0 0
Io
Figure 4.23. Lockheed compression test fixture [23]. are shown schematically in Figures 4.24 and 4.25. The specimen in Figure 4.24 is referred to as the edgewise compression test specimen and is used to determine Ey and Vyx from the initial linear portion of the loaddisplacement curves generated during testing. The applied load is assumed to be distributed equally between the top and bottom specimens. The core is assumed to carry no inplane load and is intended to supply lateral stability so that the potential for buckling is reduced. The elastic modulus and Poisson's ratio are determined from strain gage readings to be ex try P P VyxEy = ~ = = (4.19) ey ey 2Aey 2bhey
b
'
I s, ra, n g gos
P/2
core
P/2
7 Y P/2
h
x
P/2
h
Figure 4.24. Sandwich beam edgewise compression test configuration [1]. The specimen in Figure 4.25 is somewhat different because it is loaded in fourpoint bending. The specimen is the top sheet, which experiences compression. The bottom face sheet is in tension and is metal. Since the sandwich beam is subjected to flexure, various parameters (metal face sheet Strength, core cell size, etc.) can be changed to achieve the desired compression failure of the specimen [24, 25]. Poisson's ratio for this specimen is determined from direct strain gage readings to be vxy = ey/ex. The elastic modulus Ex is somewhat harder to establish since it requires an assumption of uniform deformation in each face sheet while bending
120
Laminar Composites
pecimen
Y~
~b
strain gages x i' metal
face
P/2
P/2
plate
Figure 4.25. Fourpoint bend sandwich beam compression test [1].
stresses in the core are neglected. The approximation of Ex is PL
Ex = 4bhex(2t + h + h')
(4.20)
4.3.3 Shear Tests The material properties in the plane of lamination (12) are commonly termed inplane, while those in the 13 and 2  3 planes are known as interlaminar properties. As with extensional and compressive properties, the inplane (12) properties are generally of more interest for classical laminated analysis than intedaminar properties. Five commonly accepted methods for inplane shear testing are presented next. One of these procedures contains discussions applicable to intedaminar properties. The short beam shear test, commonly used to define interlaminar shear strength, is discussed in Section 4.3.4. Discussions regarding the crossbeam sandwich, picture frame panel, and slotted tension test procedures for establishing shear properties are not considered herein, but may be found in various articles, including Lee and Munro [26]. In each of the test methods discussed, strain gages are typically used. 1. Torsion. Torsion of round specimens produces a state of pure shear, which is optimum for determining the inplane shear modulus. Two types of round specimens, either a solid rod or hollow tube, can be used.
Solid Rod. This specimen consists of a unidirectional rod, generally machined from a square bar. The shear stress distribution in this type of specimen is known to vary linearly with distance from the center of the specimen according to r = Tp/J, where T,/9, and J are the applied torque, distance from the rod center, and polar area moment of inertia, respectively. Knowing the applied torque allows for a simple prediction of stress on the outside surface of the rod. Using strain gages to determine the shear strain as a function of applied load gives a simple procedure for developing a r  y curve. The solid rod configuration is not used too often for two reasons: (1) A typical loaddisplacement (Tq~) diagram has a large region of nonlinear response, and therefore, only a limited region of the curve provides useful data; and (2) a solid specimen is expensive and difficult to produce.
Mechanical Test Methods for Lamina
121
Hollow (ThinWalled) Tube. This specimen configuration is the most desirable from a mechanics viewpoint, since the shear stress is approximately constant over the wall thickness [27]. The actual variation of shear strain from the inner to outer surfaces of the specimen can be evaluated using strain gages applied to both surfaces. Proper application of a gage to the inside surface is difficult. A single element gage oriented at 45 ~ to the axis of the specimen (Figure 4.26) provides a simple analysis tool for defining shear strain since Yxy = 2e45. As an alternative to the single element gage, a biaxial rosette can be used. The biaxial rosette should be applied so that each sensing element is at 45 ~ to the axis of the specimen (Figure 4.26). The strains indicated by the +45 ~ and  4 5 ~ gages should be equal in magnitude, and opposite in sign. The shear strain is the summation of the individual readings. A third possibility is a rectangular rosette applied so that the gages are oriented as indicated in Figure 4.26. The 445 ~ gages provide the same information as the biaxial gage, while the gage aligned with the axis of the tube provides a measure of the extent to which pure torsion is achieved. This gage should indicate no strain, or a very small strain which remains constant with increasing torque. Although axial strains are not uncommon because of compressive end forces exerted on the specimen by the torsion machine, they should be small and relatively insignificant when compared to the shear strains.
uniaxial gage
biaxial rosette
rectangular rosette
Figure 4.26. Strain gage orientations on torsion specimens.
The approximately constant throughthewall shear stress in the hollow tube specimen produces a good lry curve. Two problems associated with this test procedure are the expense of producing a hollow thinwalled tube, and the fact that a tube can be crushed by the end loads required to secure it to the torsion machine. One acceptable approach to gripping has been presented by Hahn and Erikson [28], and is schematically shown in Figure 4.27. This configuration attachment to torsion machine
\
~
r/////:
pinhole~ ~   \ tube Figure 4.27. Grips for torsion testing composite tubes [28].
adhesive
122
LaminarComposites
provides a rigid base for clamping and adequate load transfer through pins and glue to the thinwalled torsion specimen. Variations to this adaptive end configuration are easily devised. The wall thickness to diameter ratio should generally be less than 0.030 to ensure a uniform stress distribution. 2. Shear Rail Test. The shear rail test is easier to prepare and conduct than the torsion tests. There are two acceptable configurations for the shear rail test: tworail and threerail. A schematic of the load fixture for each is shown in Figures 4.28 and 4.29, respectively. Both configurations are attributed to the ASTM D30 committee. The specimen is simple to construct and machine. The suggested overall dimensions and hole sizes for both the two and threerail specimens are shown in Figure 4.30.
t
T
P
I P
apparatus
~
specimen
Figure 4.28. Tworail shear apparatus and specimen.
P
.
apparatus~ ~
[J
,
I__1
001
0
t..
lli"= ill
m
specimen
0
C);
T,, I
strain gages
Figure 4.29. Threerail shear apparatus and specimen [1].
Mechanical Test Methods for Lamina
1.750" 0.625" 0
0
5.375" ~
12.00" o 0.500" Dia
I
(typ) _I_.~00"
0
0
I ~176"P'
123
l
(~
0.500" Dia
(typ) O
0
0
0
O
0
0
0
1.500"
6.00"
1
3.00"
2.6875"
2Rail
0.6875"
3Rail
Figure 4.30. Specimen geometry for two and three.rail shear tests [26].
For both the two and threerail configurations the shear stress in the strain gaged region of each specimen is defined in terms of the applied load P and the specimen thickness (h), as well as the distance between each vertical rail (b). The shear stress for each configuration is approximated by P
rxy = ~
P rxy = 2bh
(tworail) (threerail)
Because of the method of load application, free surfaces at the top and bottom of each specimen experience large normal stresses concentrated at the comers [29]. A lengthtowidth ratio of 10:1 has been shown to approximate a state of pure shear stress, provided the edges are perfectly clamped. The requirement of perfect clamping can be met if the bolts in the rails each apply the same clamping pressure to the edges. Since a state of pure shear is only approximated with the two and threerail configurations, a single element strain gage oriented at 45* to the load axis may not adequately define the true state of strain. 3. 10" OffAxis Test. An offaxis test is generally performed in order to establish stressstrain responses in directions other than the principal material directions. The offaxis test is a tension test and no special fixtures or specimen preparation is required. Consider the unidirectional test coupon loaded as shown in Figure 4.31. The rectangular rosette in this figure is not required for establishing G12. Its presence is solely for the purpose of indicating that an offaxis test can be used for defining more than one parameter. The strains indicated by each gage in the rosette are related to Cartesian ( x  y ) strains by the strain transformation relations in Chapter 2. The relations between gage strain and the Cartesian strains are ex = CA, ey = ec, and Yxy = 2eB  eA  ec, where CA, eB, and ec are the strains indicated by gages A, B, and C, respectively.
124
Lmcdm~ Composites
t, v
X
Figure 4.31. Off.axis test specimen. The normal stress trx and strain ex (from strain gage measurements) are related by Ex = trx/ex. Ex is a function of fiber orientation, shown in equation (3.19) as 1 Ez

m4 El
(
+
1 GI2
)
§ n4
2v12 m2n2 Ei
E2
Assuming that El, E2, and I)12 are known, and that Ex is defined from testing the specimen of Figure 4.31, the only remaining unknown is G I2, which can be determined from the foregoing equation. The uniaxial state of stress results in a biaxial state of strain in the specimen. Chamis and Sinclair [30] deduced from theoretical and experimental results that the best angle for establishing Gl2 is 10~ The 10~ angle was chosen since it minimizes the effect of longitudinal and transverse tensile stress components trl and tr2 on the shear response. A comparison of the 10~ offaxis procedure with other approaches has shown it to produce reasonable results for inplane shear properties [31]. The simplicity of the 10~ offaxis test for establishing GI2 should not be taken for granted, since problems can result from the specimen being orthotropic. A uniaxial tensile stress in an orthotropic specimen can result in a shearcoupling deformation as shown in Figure 4.32a. Constraints imposed on the specimen by rigid clamping forces at the ends (Figure 4.32b) impose other testing difficulties [32]. Clamping at the end of the specimen prohibits localized rotation and produces a nonuniform strain field. A uniform strain field can be developed at the center of the specimen provided L/w is sufficiently large [32]. The specimen
I I I I I I I I I
/
A
(a)
(b)
Figure 4.32. Effects of end constraints on off.axis tensile specimens.
Mechanical Test Methods for Lamina
125
length is considered to be the region between end tabs. The effect of shear coupling can be defined by the shear coupling ratio, rlxy = ~'xy/ex. It can be shown that rlxy is a function of the stiffness matrix such that $16 r/xy ~ii
[
3 w 2 1+ 2(L)
(
)]
$66 (S16~ 2 ~Hll ~ ~ , ]
The relationship between the apparent modulus E* (established during testing) and the actual modulus Ex is Ex = (1  ~7)E* (4.21) where
1[
rl = ~ll 1 3S66 + 2SII (L/w) 2
]
As L / w increases, r/decreases and Ex approaches E*. The actual value of (L/w) at which one can assume the shear coupling to be negligible is dependent on the material system and fiber orientation being considered, as well as on the tolerable error. 4. losipescu Shear Test. The Iosipescu shear test [33] is similar to an antisymmetric fourpoint bend (AFPB) test method for composites [34]. The major difference is that for the Iosipescu test, the shear force through the test section is equal to the applied load. The Iosipescu test fixture and specimen are shown in Figure 4.33. This test procedure can be applied to composites for determining material properties in the 12, 23, and 13 directions [35]. The appropriate fiber orientations for determining inplane and intedaminar properties are shown in Figure 4.34. This test method is versatile and allows for determination of a wider variety of material properties than other procedures. Analysis of the procedure has led to the evolution of several specimen and fixture geometries. The University of Wyoming Iosipescu test specimen and fixture [36] is commonly accepted as producing reliable results. Techniques for specimen preparation and modified testing procedures to eliminate variability of results have been introduced by Lee and Munro [37].
Figure 4.33. Schematic of losipescu test fixture and specimen [35].
126
Laminar Composites
Inplane shear stresses (21 and 12 plane) , ,
/!
_
Interlaminar shear stresses 13 and 23 planes (20 lamina)
31 and 32 planes (5 lamina) I ........ ::._!_~_ .........
A
A
Figure 4.34. Specimen configurations for determination of shear properties from the losipescu test procedure [35]. 5. [l45]zs Coupon Test. This procedure involves a uniaxial tension test of a [=t=4512s laminate, with strain gages. Although a biaxial rosette is sufficient, a threeelement rosette provides additional information that can be used to verify the state of stress in the specimen. Specimen preparation and testing are identical to a conventional tension test. A complete discussion of this procedure will not be presented at this point since the specimen is a laminate. Further discussions of this procedure are deferred until laminate analysis procedures are established in Chapter 6. Results from the [=i=4512s test are in good agreement with those from other procedures, and it is considered to be a reliable test configuration.
4.3.3.1 Summary of Shear Test Methods A definitive conclusion as to which of the available procedures for establishing shear properties is "best" would be difficult to defend, since some procedures work better with one type of material than another. Evaluations of several procedures [38] indicate that more than one procedure can be categorized as appropriate for defining inplane shear properties. Lee and Munro [37] attempted to evaluate nine experimental procedures for determining inplane shear properties. They established 11 criteria within four broad categories relating to a successful experiment. These categories are fabrication cost, testing cost, data reproducibility, and accuracy. Each criterion was rated from 0 to 10, with 10 the highest, and a weighting function was applied to each. Both the rating and weighting functions of each criteria are subject to author preference. Table 4.1 presents the raw score and overall rating for each method discussed in Adams and Walrath [36]. Three
Mechanical Test Methods for Lamina
127
of the procedures presented in Table 4.1 have not been discussed herein, but can be found in the archival literature relating to composite materials testing. Table 4.1. Evaluation of inplane shear test methods [37]. Test Procedure Raw Score Tworail shear Threerail shear [+45]s 100 offaxis Crossbeam Picture frame Thinwalled tube Slottedtensile Iosipescu ,
Rating
6880 7200 8030 7860 5890 6650 6530 6990 8030 ,
6 4 1 3 9 7 8 5 1 ,
4.3.4 Flexure Tests There are two commonly used loading conditions for flexure testing: threepoint and fourpoint bending. Each is shown schematically in Figure 4.35 with the general specimen geometry. The L/4 load reaction position in the fourpoint bend configuration is sometimes replaced by an L/3 reaction position. The L/4 location is generally used with highmodulus materials (graphite/epoxy, boron/epoxy, etc.). The objective of these tests is to determine flexure strength and material modulus in specific directions. These tests are not recommended for generating design data. The flexure test can be used to determine interlaminar shear properties.
,~
tvf ~ L~
., Specimengeometry ' L
=1
lO O.O,O
~P ~~ L/2
~
Fiberorientationsfor determining dirfferentel E , a:stic/m~/ E 2'f/
1
,,
L/4 a=,.._ I ~ , , ~ l l W
3pointbend
"
I r
O ......
L/2
.,,
4pointbend
Q
S
! I~. x
Figure 4.35. Schematic of three.point and fourpoint bend tests.
Requirements for specific types of flexure tests (specimen dimensions, loading rate, etc.) are given in ASTM D79071. Unidirectional specimens with fibers oriented at either 0 ~ or 90 ~ to the beam axis can be used to determine the elastic modulus
128
Laminar Composites
of a material. The modulus along the beam axis of the specimen is generally designated as Ex, and, depending upon fiber orientation, corresponds to E1 or E2. The appropriate fiber orientations corresponding to estimates of El and E2 for flexure specimens are shown in Figure 4.35. The recommended span to depth ratio, L/h, for a flexure specimen depends on the ratio of tensile strength parallel to the beam axis and interlaminar shear strength. For 0 ~ specimens with a strength ratio less than 8:1, the recommended L/h ratio is 16. For highmodulus materials (such as graphite/epoxy or boron/epoxy) an L/h ratio of 32 is suggested. The requirement on a 90 ~ lamina is less severe, and L/h = 16 is generally acceptable for all materials. Estimating the modulus for 0 ~ or 90 ~ specimens requires knowing the deflection (w) of the center of the beam. Given the beam width (d), center span deflection (w), applied load (P), and beam length (L), the elastic modulus along the beam axis (Ex) for each configuration can be determined from strength of materials techniques. For the fourpoint bend specimen the deflection at midspan (x = L/2) is Exlw = 11PL3/768. For a beam with crosssectional dimensions as shown, I = bh 3. This results in the elastic modulus for the beam being expressed as Ex = 11PLa/64bh3w. A similar approach is used for the threepoint bend specimen. If shear deformation is considered, these equations contain an additional term. The predicted elastic modulus for each configuration (including shear deformation) are as defined in Whitney et al. [ 1]:
pL 3 Ex = 4bh3 w (1 + S)
(threepoint bend)
pL 3 Ex = 64bh3~ (11 + 8S)
(4.22) (fourpoint bend)
where S is the shear correction factor, which is a function of specimen geometry and deformation. General definitions of the shear correction factor are found in many strength of materials texts. For a rectangular crosssection the expression for S is
S=
3h2Ex 2L2Gx~
In this expression Gxz is the shear modulus in the longitudinal plane through the thickness of the specimen. It is difficult to determine and in many cases is not adequately known. It can be neglected by allowing the shear correction factor (S) to be set equal to zero, thus reducing the preceding equations to a simpler form. With S = 0 each of these expressions is a simple function of (L/h) 3. In order to estimate Ex, a series of tests with increasing L/h ratios of the specimen are conducted. The modulus Ex for each test is computed, and when a constant Ex is obtained between several test specimens, the modulus is considered to have been determined. An additional type of flexure test is the short beam shear test. Unlike the flexure tests, this test is designed to estimate intedaminar shear strength only. There are difficulties associated with it, and its overall value is questionable. The procedure and specimen dimensions for this test are discussed in ASTM D234476. The
Mechanical Test Methods for Lamina
129
specimen should be designed so that shear deformation effects are as large as possible, and failure results from interlaminar shear stresses rather than normal stresses. The ratio L/h should be small (L/h = 4 is suggested for graphite/epoxy), and a threepoint bend test is used. The specimen has a parabolic shear stress distribution through the thickness, and the maximum shear stress may not be at the midsurface of the beam. For the short beam shear test the interlaminar shear strength is expressed as 3p "rm = 4bh
(4.23)
where lrm is the maximum intedaminar shear stress, P is the applied load, and b and h are the beam width and thickness, respectively.
4.3.5 Failure Strengths The failure strengths of unidirectional composites (lamina) can be determined from the same tests used to estimate moduli. The failure strengths in the principal fiber directions require both tensile and compressive tests. Shear strength, on the other hand, is independent of load direction.
4.4 Physical Properties The physical properties of a composite material system can be as important as mechanical properties in assessing suitability for a particular application. The properties of most practical interest from a stress analysis point of view are density, fiber volume fraction, and coefficients of thermal and hygral expansion. The general procedures used to estimate these properties are highlighted in this section.
4.4.1 Density The density can be determined by first preparing a specimen with a volume on the order of v > 1 cm 3 (0.061 in3). The procedure for estimating density is: 1. Accurately determine the specimen dimensions. 2. Weight the specimen in air. The weight of the specimen in air is designated as a. 3. Weigh the specimen in water while suspending it by a wire. As part of this step, the weight of the wire (used to suspend the specimen) and the sinker (used to ensure that the specimen is submerged) must be taken into account. Therefore, two additional terms must be accounted for: w, the weight of sinker and immersed wire, and b the specimen weight +w. 4. Calculate the lamina density in mg/m 3 from p=
0.9975a a+wb
where 0.9975 is a conversion factor from specific gravity to density. A complete description of this procedure can be found in ASTM D79266.
130
Laminar Composites
4.4.2 Fiber Volume Fraction In order to estimate the volume fraction of fibers in a given specimen, a series of tests is required. Results from some of these tests are sensitive to measurements taken during the experiment. The procedures to be followed are based on the assumption that a small specimen has been prepared from a larger sample of the lamina under investigation. The general procedures are: 1. Determine the weight of the composite sample (Wc) and its density (Pc) as described in the previous section. 2. Allow the matrix to be digested either by an acid bath or by burning it away. The appropriate procedure is dictated by the fiber material. Graphite fibers, for example, require acid digestion, while glass fibers can be burned. 3. After the matrix is removed, only the fiber remains. The fiber weight (Wf) and density (pf) must then be determined from procedures established in Section 4.4.1. The volume fraction of fiber is then estimated from
~f
Wf/pf Wr162
Similar procedures can be used to determine the volume fraction of voids. The mass fractions of fiber and matrix, and their respective densities are required to compute Vv. Slight errors in measurements can lead to significant errors in estimates of volume fractions. In estimating Vv the relationship developed in Section 3.4 is useful: vv=lp
[mf ] ~+mm Pf
Pm
4.4.3 Thermal Expansion and Moisture Swelling Coefficients Coefficients of thermal expansion can be determined by using a dilatometer, or strain gages. A dilatometer measures the elongation of a specimen subjected to either high or low temperatures. The strains in the x and y directions (which could represent the 1 and 2 directions of a lamina) can be determined by ex = A x / b and ey = A y/a, where Ax and A y are specimen deformations recorded by deflection gages, and a and b are the lengths of each side. The strains could alternatively be measured from strain gages. Each strain is plotted as a function of temperature. The slope of the resulting curve in the linear portion of the graph is taken to represent the coefficient of thermal expansion t~, as illustrated in Figure 4.36. Different expansion coefficients can be observed during heating and cooling cycles of a test sequence. The moisture swelling coefficients are determined in a manner analogous to that for estimating thermal expansion coefficients. By measuring the volume change in a specimen as a function of moisture weight gain, a plot similar to Figure 4.36 can be established for moisture. The slope of the resulting curve represents the coefficient
132
0
0
~
0
I
t~
tt~
I ~176176
v.~ v  4
t'~l cr~ fr
,.~
0
0
0
v.~
0
v4
cr~
v.~
cr~ ce~ or1
t',,I ,, ,* ce~ f',l
~
0
Laminar Composites
~t
r~ t~
el,
f,4 or3
t"4
'
IIII
IIII II
II II
II
I I
O ~ t"4
t ' 4 ,,
cr~ cr~
,  , 0 0 0 ,"~ , "
0
9, t ' ~ ,~ c 4
0
t~t ~
O 0
0
~D~
O 0
~
~
t._.J ~..J
,~ ,,
t._.J ~..J
t',4 cr~
ce~ ,~
.
9  , 0
f ' 4 ,* ~
~
c,40
...4
o
0
0 up3 ....4
i
0 0
II
O 0
::L
0
0 U 0
~0 0
0
r~
for LmMaa
II
Test Metkods
IIII !1
Mechanical
Illll I!
O 0
o.o.
I
I III 0
0 0 0 0
o.o.
o.o
0
oc~o
oo.
I
Jtlll
0
I
o
o ~ o
o~.o.o.o.o
o.
o.
o.~ooo,
dc~
o.o
c~d
~.q
~.~.
qq
.
~.
t',,I eel
oo
~
or.
~
9~ ,~ ~ t.
m.e.:.~,
9 ~.~.
c~ c ~ c ~ c ~
c~
o.o
0
o o o
0,.~ 0
o
.
o.v!.oo.o.o.
000 0 0 0 0 0 0
~ ~ o ~ oo,.., ,
o.o.o.o.o.o.
c~c~c~c~c~c~
00
133
134
m
.m
!"•
k~
a
O.
.~0 t',l
e~ rq e  ~
0,4(",11
O 0
9
I
tt3 0
9
t"4 Cr~
O 0
~
cr~ t ~
0 . 0
I I I I !
'q'
Laminar Composites
l t.__
0
I
.'q"
C~I ~
tt~
I I I I I
t',4 t ~
e..~ e~ .q e~ e.q
z
oo
q
o.o
I~7
~.~.
177
d
tt3
o
U'3 ~D
o
t.
d d
d~
d
d
1111111
e..q e~ e.~ e~ .  . q e  ~ e  ~
m~
,m
.,
o
I
,,
o o
~d
0
9
IIIII
q
I~
ITI
d
I
o'
o
I~I d
~i ~ 
IIIIIII
~, d ~ d d
Mechanical Test Methods for Lamina
NI I l
~
IIIII
qqqqq
0
C ~ O 0 0 0
135
136
Laminar Composites
4.6 Testing Lamina Constituents
Complete characterization of a composite material includes fiber and matrix properties. Both physical and mechanical properties are determinable in many cases. Because the constituent materials are typically isotropic, some of the complexities of testing orthotropic lamina are reduced, while some tests applicable to lamina are not appropriate for the constituents. For example, compression testing of single fibers cannot be accomplished. Tensile testing of fibers, however, is a wellestablished procedure as discussed in detail in ASTM D337975. Special test fixtures, such as the one schematically shown in Figure 4.37, as well as data reduction procedures are required for testing fibers. wax
~
specimen
 fixture
. . . . .
i
I
f
~o
i ,,..
Figure 4.37. Schematic of testfixture for fibers. Since fibers can only be tested in tension, the basic properties generally established for resin systems are tensile. The procedures for testing different polymeric resin systems depend on the availability of the material as either a thick sheet or thin film. The test procedures and specimen configurations for thick sheet forms of material are detailed in ASTM D63872. Similar information corresponding to thin film material is available in ASTM D88273. An appropriate procedure for characterizing them depends on their general classification as elastic, plastic, viscoelastic, etc. Tables 4.4 and 4.5 present a range of values for some of the physical and mechanical properties of selected fibers and resins systems in English and SI units, respectively. 4.7 References
1. Whitney, J. M., I. M. Daniel, and R. B. Pipes. Experimental Mechanics of Fiber Reinforced Composite Materials. SESA Monograph No. 4. Westport, CT: Technomic, 1982. 2. Carlson, L. A., and R. B. Pipes. Experimental Characterization of Advanced Composite Materials. Englewood Cliffs, NJ: PrenticeHall, 1987. 3. Pendleton, R. L., and M. E. Tuttle. Manual on Experimental Methods of Mechanical Testing of Composites. Westport, CT: SEM, 1990. 4. Dally, J. W., and W. F. Riley. Experimental Stress Analysis. New York: McGrawHill, 1978. 5. "Student Manual for Strain Gage Technology," Bulletin 309, Measurements Group Inc., P.O. Box 27777, Raleigh, NC. 6. "Surface Preparation for Strain Gage Bonding," Bulletin B1295, Measurements Group Inc., P.O. Box 27777, Raleigh, NC.
Mechanical Test Methods for Lamina
137
7. Perry, C. C., and H. R. Lissner. The Strain Gage Primer, 2nd ed. New York: McGrawHill, 1962. 8. "Optimizing Strain Gage Excitation Levels," MM Tech Note TN502, Measurements Group Inc., P.O. Box 27777, Raleigh, NC. 9. "Standard Test Methods for Performance Characteristics of Bonded Resistance Strain Gages," ASTM Standard E25167. 10. "Errors Due to Transverse Sensitivity in Strain Gages," MM Tech Note TN509, Measurements Group Inc., P.O. Box 27777, Raleigh, NC. 11. Tuttle, M. E. "Error in Strain Measurement Obtained Using Strain Gages on Composites," Proc. 1985 SEM Fall Mtg., Nov. 1720, pp. 170179, 1985. 12. Tuttle, M. E., and H. F. Brinson. "ResistanceFoil Strain Gage Technology as Applied to Composite Materials," Experimental Mechanics, 24 (1984): 5465. 13. McCalvey, L.F. "Strain Measurements on Low Modulus Materials," presented at BSSM Conference, University of Surrey, U.K., Sept. 1982. 14. White, R. N. "Model Study of the Failure of Steel Structures," Presented at ASCE/SESA Exchange Session on Physical Modeling of Shell and Space Structures, ASCE Annual Convention, New Orleans, LA, 1982. 15. Steklin, P. "Strain Distribution in and around Strain Gages," J. Strain AnaL, 7 (1972): 228235. 16. Beatty, M. F., and S. W. Chewning. "Numerical Analysis of the Reinforcement Effect of a Strain Gage Applied to a Soft Material," Int. J. Eng. Sci., 17 (1979): 907915. 17. E1Tahan, W. W., G. H. Staab, S. H. Advani, and J. K. Lee. "Structural Analysis of Bimodular Materials," ASCE J. Eng. Mech., May (1989): 963981. 18. Schoeppner, G. A., and R. L. Sierakowski. "A Review of Compression Test Methods for Organic Matrix Composites," J. Composites Technology & Research, 12 (1990): 312. 19. Hofer, K. E., Jr., N. Rao, and D. Larsen. "Development of Engineering Data on Mechanical Properties of Advanced Composite Materials," AFMLTR72205, Part I, Sept. 1972. 20. Verette, R. M., and J. D. Labor. "Structural Criteria for Advanced Composites," AFFDL TR 76142, Vol. 1. Summary, March 1977. 21. Kasen, M. B., R. E. Schramm, and D. T. Read. "Fatigue of Composites at Cryogenic Temperatures," Fatigue of Filamentary Composites, ASTM STP 636, K. L. Reifsnider and K. N. Lauraitis, eds. Philadelphia: ASTM, pp. 141151, 1977. 22. Grimes, G. C., P. H. Frances, G. E. Commerford, and G. K. Wolfe. "An Experimental Investigation of the Stress Levels at Which Significant Damage Occurs in Graphite Fiber Plastic Composites," AFMLTR7240, May 1972. 23. Ryder, J. T., and E. D. Black. "Compression Testing of Large Gage Length Composite Coupons," Composite Materials: Testing and Design (Fourth Conference), ASTM STP 617. Philadelphia: ASTM, pp. 170189, 1977. 24. Lantz, R. B., and K. G. Baldridge. "AnglePlied Boron/Epoxy Test Method~ A Comparison of BeamTension and Axial Tension Coupon Testing," Composite Materials: Testing and Design, ASTM STP 460. Philadelphia: ASTM, pp. 94107, 1969. 25. "Uniaxial Compression," Section 4.2.4, Advanced Composites Design Guide, Vol. 4. Materials, 3rd Ed. Air Force Flight Dynamics Laboratory, Dec. 1975.
138
Laminar Composites
26. Lee, S., and M. Munro. "Evaluation of InPlane Shear Test Method for Advanced Composite Materials by the Decision Analysis Technique," Composites, 17 (1986): 1322. 27. Whitney, J. M., and J. C. Halpin. "Analysis of Laminated Anisotropic Tubes under Combined Loading," J. Comp. Mtl., 2 (1968): 360367. 28. Hahn, H. T., and J. Erikson. "Characterization of Composite Laminates Using Tubular Specimens," AFMLTR77144, Aug. 1977. 29. Whitney, J. M., D. L. Stansbarger, and H. B. Howell. "Analysis of the Rail Shear TestApplications and Limitations," J. Comp. Mater, 5 (1971): 2435. 30. Chamis, C. C., and T. H. Sinclair. "TenDegree OffAxis Test for Shear Properties in Fiber Composites," Exp. Mech., 17(9) (1977): 339346. 31. Yeow, Y. T., and H. F. Brinson. "A Comparison of Simple Shear Characterization Methods for Composite Laminates," Composites, 9 (1978): 4955. 32. Halpin, J. C., and N. J. Pagano. "Influence of End Constraint in the Testing of Anisotropic Bodies," J. Comp. Mtl., 2 (1968): 1831. 33. Iosipescu, N. "New Accurate Procedure for Single Shear Testing of Metals," J. Mater., 2(3) (1967): 537566. 34. Slepetz, J. M., T. F. Zagaeski, and R. F. Novello. "InPlane Shear Test for Composite Materials," AMMRC TR 7830, Army Materials and Mechanics Research Center, Watertown, MA, July 1978. 35. Walrath, D. E., and D. F. Adams. "The Iosipescu Shear Test as Applied to Composite Materials," Exp. Mech., 23(1) (1983): 105110. 36. Adams, D. F., and D. E. Walrath. "Further Development of the Iosipescu Shear Test Method," Exp. Mech., 27 (1987): 113119. 37. Lee, S., and M. Munro. "Evaluation of Testing Techniques for the Iosipescu Shear Test for Advanced Composite Materials," J. Comp. Mater., 24 (1990): 419440. 38. Lee, S., M. Munro, and R. F. Scott. "Evaluation of Three InPlane Shear Test Methods for Advanced Composite Materials," Composites, 21 (1990): 495502. 39. Reinhart, T. J. Engineered Materials Handbook, Vol. 1. Composites, Materials Park, OH: ASTM International, 1989. 40. Schwartz, M. M. Composite Materials Handbook, New York: McGrawHill, 1984. 41. Beland, S. High Performance Thermoplastic Resins and Their Composites, Park Ridge, NJ: Noyes Data Corporation, 1990. 42. Tsai, S. W., and H. T. Hahn. Introduction to Composite Materials, Westport CT: Technomic, 1980. 43. Vinson, J. R., and R. L. Sierakowski. The Behavior of Structures Composed of Composite Materials, Dordrecht, The Netherlands: Martinus Nijhoff, 1986. 40 Jones, R. M. Mechanics of Composite Materials. New York: Hemisphere Publishing, 1975. 45. Ashton, J. E., J. C. Halpin, and P. H. Petit. Primer on Composite Materials: Analysis. Westport, CT: Technomic, 1969. 46. Hull, D. An Introduction to Composite Materials. New York: Cambridge University Press, 1981. 47. Chawal, K. K. Composite Materials Science and Engineering. New York: SpringerVedag, 1987.
Mechanical Test Methods for Lamina 4.8
139
Problems
4.1 Assume that a uniaxial strain gage is mounted on a unidirectional tensile specimen made of T300/5208 graphite/epoxy. The gage is oriented as shown and the specimen is subjected to an applied load tr0 as indicated. Determine the percent error resulting from neglecting transverse sensitivity for (A) K   0 . 4 0 %
(B) K    1 . 5 % ,
,
I
,,,,
v
~0
,==
,,,

i
i
i
a0
_ .
.
.
.
4.2 The strain gage of Problem 4.1 is applied to a T300/5208 graphite/epoxy specimen as indicated. Determine the percent error which results from neglecting the transverse sensitivity for (A) K = 0 . 4 0 %
(B) K =  1 . 5 %
o iIH IllllIII!iil I !illl 4.3 A uniaxial strain gage is used to measure the maximum tensile strain on the outside surface of a closedend pressure vessel subjected to an internal pressure P. The vessel is made from a unidirectional graphite/epoxy (AS/3501) with its fibers oriented along the longitudinal axis of the vessel. Determine the percent error resulting if transverse sensitivity is neglected. [Hint: Determine the state of stress in the vessel using classical thinwalled pressure vessel theory.] (A) K = 0 . 4 0 %
(B) K =  1 . 5 %
4.4 The results from a uniaxial tension test on AS/3501 graphite/epoxy are presented below. Find El, E2, Vl2, vl2, X, and Y. 250 I i ! ' I ~ ~ i i I I'= , ,
10
200
8
~"
150
~"
6
~
100
~
4
50
2
0
0 0
5000
10,000 15,000
Axial Strain (llin/in)
0
5000
Axial Strain (pin/in)
10,000
140
Lamdam
Composites
4.5 The fourpoint bend sandwich beam compression test is schematically shown in Figure 4.25. In the region of the beam where the bending moment is constant, the forces in both top and bottom layers can be modeled as shown. The bending moment at section A  A in this section can be expressed in terms of the applied load P and the beam length L. (A) Determine the relationship between Fl, FE, t, h, h', and the bending moment at section A  A expressed in terms of P and L. (B) Assuming that F I = Fe, determine the expression for Ex which is known to be
PL Ex = 4bh(2t + h + h')ex
=,.~\\t~ 2 P/2
////
A jh
,, ct , ....... II I_~l ,
.......
\ P/2
/
x
~'""
/ 1k! !
I ~'"'~
;.?
wT'f/'r
FA"'~2' M
,,.._
P/2 r
4.6 The Iosipescu shear test is schematically shown in Figure 4.33. A schematic of the loads that the fixture transmits to the specimen is shown in Fig. A; a schematic of the loads experienced by the specimen is shown in Fig. B. (A) Use Fig. A to verify that PI = P a / ( a  b) and P2 = p b / ( a  b). (B) Use Fig. B to show that the specimen test section (the vertical plane through the notch) experiences a shear force equal to the applied load P and no bending. P~
Fig. .... A
Fig. B
~P2 _
_
~P1
_
_
P2
~
"
!
h
9rip 2 4.7 A schematic diagram for the asymmetrical fourpoint bend (AFPB) shear loading fixture [34] is shown below. For this test configuration, verify that the shear force in the specimen test section (the vertical plane through the notch) is given as ab V = p ~ a+b
Mechanical Test M e t ~
.
141
P . ~ L b/2 .=
a/2
c~
for Lamtaa
.
,
(i,/#"
.~
f
i
,=r~ r /
/
!
L
#" /
J
/'~"
b/2
"/..1
J.
t"
/
a/2
4.8 Experimental data from thermal expansion tests are presented below for three types of materials. From this data, determine the coefficients of thermal expansion for each material. 20000
',
'i
,
if,',
,
,
[ i ,
,"' i ' " l
t"i
i
'
I
'
i
,
il
'
i
,
,
[,
,
i
rl
i
i
o
i

15000 Ar ~ r
r
Kevlar 1direction K e v l a r 2direction S  G l a s s 1direction S  G l a s s 2direction G r a p h i t e 1direction G r a p h i t e 2direction
Oz~ 'El
10000 " 5 0 0 0 _
_ _ .
I
I
a I
I
I
I
Ill
~
100
I
I

i

I

~ r.~~
J


._._.
9
i
,
_~
~
_
i
c
;..l
J I
_
_
I
.... I
200 T e m p e r a t u r e (~
I
I
I
~
= i
9
I
_

300
I
I
i
I
I
I
i
i
I
400